Manufacture and properties of sand-lime brick.
Embed Size (px)
Transcript of Manufacture and properties of sand-lime brick.
DEPARTMENT OF COMMERCE
Technologic Papersof THE
Bureau of StandardsS. W. STRATTON, Director
MANUFACTURE AND PROPERTIES OFSAND-LIME BRICK
WARREN E. EMLEY, Associate ChemistBureau of Standards
ISSUED MARCH 22, 1917
WASHINGTONGOVERNMENT PRINTING OFFICE
ADDITIONAL COPIESOF THIS PUBLICATION MAY BE PROCURED FROM
THE SUPERINTENDENT OF DOCUMENTSGOVERNMENT PRINTING OFFICE
WASHINGTON, D. C.AT
10 CENTS PER COPY
A complete list of the Bureau's publicationsmay be obtained free of charge on applicationto the Bureau of Standards, Washington, D. C.
MANUFACTURE AND PROPERTIES OF SAND-LIME BRICK
By Warren E. Emley
CONTENTS PageI. Introduction 3
II. History , 4III. Definition and description 5IV. Process of manufacture 6
V. Calcium silicate 6
VI. Raw materials 81. Sand 8
Delivery of sand to the factory 11
2. Lime 13Hydration of the lime 15
3. Proportions of sand and lime 19VII. Mixing 21
VIII. Pressing 23
IX. Hardening 24X. Handling 26
XI. Properties 26
XII. Tests 271. Results of tests 28
(a) Crushing strength 28
(b) Transverse strength 30
(c) Absorption 31
(d) Freezing 32
(e) Fire test 32
(/) Miscellaneous 342. Summary 34
Appendix 381. Description of plants , 38
(a) Factory located at Spokane, Wash 38(b) Factory located at Minneapolis, Minn 38(c) Factory located at Milwaukee, Wis 39(d) Factory located at Grand Rapids, Mich 39(e) Factory located at Kalamazoo, Mich 40
(/) Factory located at Dayton, Ohio 40
(g) Factory located at Waltonville, Pa 41
After years of experimenting, fraught with numerous vicissi-
tudes, sand-lime brick has finally achieved a permanent position
as a common building material. Putting this industry on apractical paying basis has been beneficial not only to the manu-
facturers themselves but also to the general public. Almost
4 Technologic Papers of the Bureau of Standards
every citizen has a direct personal interest in building materials.In many parts of the country clay of the quality required to makea good brick is not to be had, and the price which can be obtainedfor common brick is generally too low to permit of shipping themany great distance. To the people residing in such localities themanufacture of sand-lime brick has been of particular advantage.Sand of a sufficiently good quality is generally abundant, especiallyin those localities where there is no clay. The ability to makebrick of the sand has placed within reach of the users a cheap,durable, noncombustible building material, which is a homeproduct with reasonable transportation costs.
sand //ire wafer
fiehime*/-*. GS% f AT% crusher
Iu r*tCC(^i/rer' r-j _gr,ncter
I (- erfgi/^fr fyf fit/a/ate //re
S//o , where hyt/ral/or? /j coftptetet/
heater, to Sreo\ op /or*rp!>
terroc/^ft to J/'re proper
rt* er Co/r^/^tencyfor pr&zzjrrc,
\ ; ..
fonferrrny cy/meter, tYfyere 6rtcfc3 are Ct/ret/'(nr/tr, ^fcart
FlG. i.Arrangement of steps in process of manufacture
The process for making brick of sand was discovered andpatented by Dr. William Michaelis in 1880. 1 It is true thatPeppel 2 recognizes sand-lime brick made by other processes,and numerous statements may be found in the literature con-cerning a ''sand-lime brick" made in New Jersey about i860.This material was really a mortar brick, being made of ordinarylime mortar, molded into shape and permitted to set. So far ascan be learned, none of these earlier processes has proved a com-
mercial success. All sand-lime brick now marketed in thiscountry are made according to the basic principles covered bythe original Michaelis patent.
Dr. Michaelis permitted his patent to lapse without exploita-
tion. Almost immediately thereafter a number of modifications
1 Process of Manufacture of Artificial Sandstone, DRP, p. 14195; Oct- 5. 1880.2 S. V. Peppel, Manufacture of Sand-Lime Brick, Ohio State Geol. Sur., Bull. No. 5; 1905.
Sand-Lime Brick 5
were patented, under which the manufacture of sand-lime brick
began. These patents, in so far as they covered modifications
of the process, have all proven to be of no value and have been
generally abandoned. They were of great value to the industry,however, for the attempt to sell the rights to use them arousedand stimulated interest in the subject.
At the present time all the sand-lime brick plants in this countryfollow the Michaelis process, which is free to anyone Yv^ho cares to
use it. Only a few patents on details of machinery are now inforce.
The first plant established in the United States was built atMichigan City, Ind., in 1901 and is still in operation. Since then
the industry has grown as shown by the following figures: 3
1903 : $155,040
1909 $1, 150, 580
1, 169, 153
1904 1910 76
1905 1911 66
1906 1912 .. 71
1907 1913 . 68
1908 1914 .
Almost all sand-lime brick are sold as common building brick,the number of face brick produced being only about 6 per centof the total. The average price for common brick in 191 4 was$5-99 per thousand, f. o. b. cars at the plant.
The history of sand-lime brick manufacture has been largelyinfluenced by the activities of the Sand-Lime Brick Association.This body comprises about 40 members in the United States andCanada. It has been in existence for 12 years and has worked
consistently to cheapen the cost and improve the quality of the
brick. The annual meetings of the association provide a forumfor the discussion of new processes and machinery, they encouragescientific investigation of the product, and are steadily working
toward the point where membership in the association will carry
with it an assurance of quality of product.
III. DEFINITION AND DESCRIPTION
Sand-lime brick, as now known to the trade, consists essentiallyof sand, which is bound together by a hydrated calcium silicate.
It has about the same hardness and porosity as common clay
3 U. S. Geol. Sur., Mineral Resources.
6 Technologic Papers of the Bureau of Standards
building brick. It is naturally white in color, or nearly so, this
being determined by the color of the sand from which it is made,although a few artificially colored sand-lime brick are being sold.
The individual specimens are much more nearly uniform in sizeand shape than clay brick of the same quality. A detaileddescription of each of the important properties will be found in
a later section headed ''Tests."
IV. PROCESS OF MANUFACTURE
The essential steps in the process of making sand-lime brick are
(i) To the sand add the required amount of thoroughly hydratedlime, mixing the two intimately; (2) add enough water to bringthe material to such a consistency that it will hold together whenmolded; (3) press the damp mixture into the desired form; (4)cure the brick by means of steam under pressure. This curingprocess causes a chemical reaction between the lime and some ofthe sand to form the calcium silicate, which acts as a bonding
agent to hold the rest of the sand together.
V. CALCIUM SILICATE
Before discussing the raw materials, it would be well to have aclear understanding of the functions which they are expected to
perform. The most important function is, of course, the produc-tion of the bonding substance upon which the strength of the brick
Michaelis, in his original patent, claimed the formation of sili-
cates which are hard and resistant to the action of air and water
by treating a mixture of 10 to 40 parts of the hydroxides of calcium,barium, or strontium and 100 parts of sand or any siliceous material
with live steam at a temperature of from 130 to 300 C.
Of course the use of barium or strontium would be too expensive
for practical consideration, so that calcium hydroxide, or hydrated
lime, is always used. Some siliceous materials other than sand,however, have found a limited application. Among these may bementioned sandy loam or siliceous clay, 4 volcanic lava, 5 etc.
However, sand is by far the principal source of silica used in this
country to make sand-lime brick.The raw materials are thus limited practically to hydrated lime
and sand. It will be noted, however, that the patent allows a
4 Benson and Herrick, Use of Fine Earths in Mortars, Jour. Ind. and Eng. Chem., 6, p. 796; 1914.5 Carmichael, Proc. Sand-Lime Brick Assn.; 1912.
Sand-Lime Brick 7
wide variation in the proportions of the ingredients, that the steam
pressure used in curing the brick may vary from 5 pounds to over1000 pounds, and that no definite duration of the steam treatment
These wide variations of allowable limits would lead one to infer
the possible presence of any number of calcium silicates. Com-mon American practice has narrowed these limits, so that the pro-portion of hydrated lime is seldom over 1 5 per cent of the sand, the
steam pressure may vary from 100 to 150 pounds, and the bricksare cured from 7 to 12 hours. Under these circumstanc